HAL Id: hal-00771744
Submitted on 9 Jan 2013
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
In-plane magnetic penetration depth in NbS2
Pascale Diener, Maxime Leroux, Laurent Cario, Thierry Klein, Pierre Rodiere
To cite this version:
Pascale Diener, Maxime Leroux, Laurent Cario, Thierry Klein, Pierre Rodiere. In-plane magnetic
penetration depth in NbS2. Physical Review B: Condensed Matter and Materials Physics (1998-2015),
American Physical Society, 2011, 84 (5), pp.054531. �10.1103/PhysRevB.84.054531�. �hal-00771744�
In-plane magnetic penetration depth in NbS2
P. Diener1, M. Leroux1, L. Cario2, T. Klein1,3, P. Rodière1 1
Institut Néel, CNRS/UJF 25 rue des Martyrs BP 166 38042 Grenoble cedex 9, FRANCE
Institut des Matériaux Jean Rouxel (IMN), Université de Nantes, CNRS, 2 rue de la Houssinière, BP3229, 44322 Nantes, France and
Institut Universitaire de France and Université J.Fourier-Grenoble 1, France
We report on the temperature dependence of the in plane magnetic penetration depth (λab)
and first penetration field (Hf ∝ 1/λ 2
ab(T ) for Hkc) in 2H-NbS2 single crystals. An exponential
temperature dependence is clearly observed in λab(T) at low temperature, signing the presence of
a fully open superconducting gap. This compound is the only superconducting 2H-dichalcogenide which does not develop a charge density wave (CDW). However as previously observed in 2H-NbSe2,
this gap ( ∆1 = 1.1 kBTc) is significantly smaller than the standard BCS weak coupling value. At
higher temperature, a larger gap (∆2= 1.8 kBTc) has to be introduced to describe the data which
are compatible with a two gap model. The superconducting gaps are hence very similar in NbS2
and NbSe2 and we show here that both of them open in the strongly coupled Nb tubular sheets
independently of the presence of a CDW or not.
In numerous strongly correlated systems, superconduc-tivity appears in the vicinity of a second electronic in-stability. These superconductors then often show devi-ations from the weak coupling BCS theory which raises the question of the interplay between the two orders1.
This question is particularly well illustrated in dichalco-genides. Indeed, in 1T-TiSe22,3, 2H-TaS24,5, or
2H-NbSe2 superconductivity coexists with a charge density
wave (CDW). In 2H-NbSe2 the charge density wave
de-velops for instance at TD = 33 K and coexists with
su-perconductivity (SC) below Tc= 7.1 K.
In parallele, specific heat, tunneling spectroscopy as well as de Haas van Alphen measurements6–10 showed
that NbSe2is characterized by the coexistence of two
su-perconducting gaps : ∆1= 1.0 ± 0.1kBTc which is much
smaller than the BCS weak coupling value (∆/kBTc ∼
1.7) and ∆2 = 2.0 ± 0.3kBTc. It was then initially
sug-gested that the CDW might be at the origin of ∆111–14.
However, scanning tunneling spectroscopy (STS) and specific heat measurements clearly indicated the pres-ence of a reduced superconducting gap (of similar am-plitude) in the NbS2 system as well15,16 showing that
this interpretation does not hold the ground. Indeed, this iso-electronic compound is particularly interesting to probe the possible influence of the CDW on the superconducting states in dichalcogenides, as it is the only system among the four 2H layered superconduct-ing transition-metal dichalcogenides17 MX
X=S, Se) which does not exhibit a CDW transition. Those measurements hence clearly showed that the pres-ence of two superconducting gaps in 2H-dichalcogenides is not a direct consequence of the presence of a CDW in some of them.
In a first scenario, those two gaps can be considered as being the limiting values of one single anisotropic su-perconducting gap (without nodes) whereas in an alter-native scenario they can be related to different values of the electron phonon coupling constants (λe−ph) on
differ-ent sheets of the Fermi surface (FS) (so called multiband superconductivity18).
Clear evidence for multiband superconductivity were first obtained in MgB2for which λe−phvaries from ∼ 1.2
for the 2D-σ band to ∼ 0.4 for the 3D-π band19,20. Since
the FS of NbSe2 is composed of four strongly coupled
quasi-2D Nb-derived cylinders (bands 17 and 18 with λe−ph ranging from 0.8 to 1.9) and one Se-derived
pan-cake sheet with a much smaller λe−ph value ∼ 0.3 (band
16)8, it was tempting to ascribe the small
superconduct-ing gap to this reduced λe−ph21,22. However ARPES
measurements11,14 suggested that, in NbSe
2, both gaps
open on the tubular sheets and the situation iseems to be quite different from that of MgB2 as the two gaps
could both be associated to the same (strongly coupled) FS sheets. However, an experimental confirmation that the tow gaps are also related to the same FS sheets in NbS2 was still lacking.
In order to address this issue, we have performed in plane penetration depth and penetration field measure-ments in NbS2 single crystals. Indeed, λ is a directional
probe and corresponding measurements are only sensitive to supercurrents flowing perpendicularly to the direction of the applied magnetic field. Band structure calculations in NbSe2have for instance shown that the tubular sheets
contribute to 98% of the transport current in the basal plane23, and the present measurements will hence only
probe the superconducting properties of those strongly couple sheets. We show here that the temperature de-pendence of λab are remarkably identical in NbSe2 and
NbS2. This temperature dependence clearly confirms the
presence of a small superconducting gap ∆1 = 1.1 kBTc
(being much smaller than the standard BCS weak cou-pling value) and that, as previously observed in NbSe2,
this gap opens on as least one of the Nb sheets. At higher temperature the superfluid density can be deduced from λ(T ) introducing a calibration factor (see below) which can be accurately obtained combining λ(T ) and first pen-etration field measurements. We then also show that a second gap value is required to describe the
tempera-ture dependence of this superfluid density which can be well described by a two gap model introducing gap values very similar to those previously obtained in specific heat measurements. We hence confirm that the presence of two well defined superconducting gap values, both open-ing on the Nb tubular sheets in a generic feature of 2H-dichalconenides.
STS and specific heat (Cp) measurements clearly
showed that NbSe2 and NbS2 systems share the
par-ticularity of having both two superconducting gaps but also highlighted some fundamental differences. Indeed, whereas vortices exhibit a clear stellar shape in NbSe2,
they appear to be isotropic in NbS2. Moreover, the two
systems have very different anisotropies of their upper critical fields increasing from ∼ 3.2 in NbSe29to ∼ 8.1 in
NbS224. However, the vortex shape and Hc2 values are
determined by the coherence length (ξ) which is related to the superconducting gap but also to electronic prop-erties of the normal state (Fermi velocity and possibly electronic mean free path in the so-called dirty limit). On the contrary the temperature dependence of the pen-etration depth is determined only by the superconducting gap structure. Those later measurements hence provide very valuable information to understand those differences which will be discussed at the end of the paper.
II. SAMPLE AND EXPERIMENTS
2H-NbS2 samples were grown using the vapour
trans-port growth technique with a large sulphur excess, as described elsewhere25. Single crystals have a flat
hexag-onal or triangular shape and typical dimensions of 1502×
30 µm. The large flat faces grow perpendicular to the c-axis. The 2H crystallographic structure has been checked on each sample using a four-circle diffractometer. The bulk critical temperature was checked on several sam-ples of each batch by ac specific heat16. All the
mea-sured crystals showed sharp superconducting transitions (∆Tc∼ 0.3 K) at Tc= 6.05±0.2 K emphasizing the
excel-lent bulk homogeneity of each crystal. Previous scanning tunnelling microscopy measurements on single crystals of the same origin confirmed the absence of CDW down to 0.1 K15. To avoid a contamination by oxygen
intercala-tion between layers which would reduce Tc and smears
the transition24, samples were kept in vacuum. All the
measurements were carried out in the first month follow-ing the growth of the samples.
A high stability LC oscillator operating at 14 MHz, driven by a Tunnel Diode26–28has been used to measure
the variation of the magnetic penetration depth. The tiny sample, placed in the center of the solenoid coil, acts as a small perturbation to the inductance (L). By chang-ing the temperature of the sample, the magnetic penetra-tion depth variapenetra-tions produce a change of the inductance, leading to a change in the LC resonant frequency δf(T ). The amplitude of the AC excitation field is smaller than 1µT (that is «Hc1) to keep the sample in the Meissner
Figure 1: Temperature dependence of the frequency shift δf (T), for B (square) D (triangle) (right scale)and C8 (cir-cle) (left scale)NbS2 single crystals. Inset: microscope images
of each sample (note the bigger scale for C8).
state. This technique enables to measure the variation of λ with an excellent sensitivity as our setup can detect relative frequency changes, δf/f0 of a few 10−9, which
corresponds to changes in λ on the order of 1 Åin mm3
samples. The sample is glued with vacuum grease at the bottom of a sapphire cold finger whose temperature is regulated between Tmin=0.5 K and 10 K whereas the
LC oscillator remains at fixed temperature (3K). The fre-quency shift δf=f(T ) − f(Tmin) is then proportional to
the magnetic penetration depth : δλ(T ) = Rδf (T )
(1) where ∆f0 is the change induced by the introduction of
the superconducting sample in the coil (measured in-situ by extracting the cold finger from the coil at the low-est temperature), and R an effective dimension which depends on the sample geometry. In principle, R can be evaluated by using the formula proposed by Prozorov and al.29 in the case of cylinders. However, recent
mea-surements in pnictides highlighted the difficulties of eval-uating this effective dimension, in particular for mag-netic fields perpendicular to the ab-planes (main sample surface)30. Indeed, very different δλ(T ) were obtained by
different groups, most probably due to the roughness of the sample edges which undermines this evaluation.
To overcome this difficulty we have performed first pen-etration field (Hf) measurements using miniature
GaAs-based quantum well Hall probe arrays. The remanent local DC field (Brem(Ha)) in the sample has been
mea-sured after applying a magnetic field Ha and sweeping
the field back to zero. In the Meissner state, no vortices penetrate the sample and Brem remains equal to zero up
to Ha = Hf. A finite Brem value is then obtained for
Ha ≥ Hf due to vortices which remain pinned in the
sample. As Hf is directly proportional to the first
cal field Hc1∝ 1/λ2, the normalized in plane superfluid density : ˜ ρab(T ) = λ 2 0 λ2 ab(T ) = 1 (1 + R λ0∆f0δf (T )/) 2 (2)
is expected to vary as Hf(T )/Hf(0) (λ0 being the zero
temperature penetration depth). Even though the un-certainties on the Hf values hinders any precise
determi-nation of the gap values, those measurements can then be used as milestones to obtain the R/λ0∆f0 coefficient
(see inset of Fig.3).
III. EVIDENCE FOR A SMALL GAP VALUE IN
Fig. 1 shows typical δf(T ) curves between 0.08 Tc
and 0.85 Tc for three NbS2 single crystals (see inset of
Fig. 1). The magnetic field is applied perpendicularly to the layers, i.e. along the crystallographic c axis, so that supercurrents are flowing in the layers, probing the in-plane penetration depth, λab31. Samples B and D were
grown in the same batch, and have, in-plane dimensions equal to 110 µm and 140µm, respectively and a thick-ness t = 30µm (resp. 25µm). Sample C8 was grown in a second batch and has a larger size (4302× 110 µm3).
The frequency shift is ten times higher for C8 than for other samples due to it larger volume but all renormal-ized curves are fully identical underlying the excellent reproducibility of the temperature dependence discussed below.
In the local London theory, at low temperature (typi-cally T < Tc/3), the temperature dependence of the gap
can be neglected and λ(T ) is given by : (λ(T ) − λ0)/λ0=
where kB is the Boltzmann constant and ∆(0) the value
of the smallest superconducting gap at 0 K. Indeed, due to this exponential dependence only the smallest gap is expected to show up at low temperature. As shown in Fig.2 a very poor agreement to the data is obtained if the gap parameter is fixed to the weak coupling BCS gap of 1.76kBTc. A much better fit is obtained taking
∆/kB = 7.2 K≈ 1.2 Tc. Note that this gap value does
not depend on the renormalization constant. The as-sumption λ(Tmin) ≈ λ0, where Tminis the lowest
exper-imental temperature, is valid here, since an extrapolation of Eq.(3) gives (λ(0.5K) − λ0)/λ0< 10−3. Since the
su-perfluid current mainly originates from the Nb sheets for Hkc, those measurements hence directly show that this small gap is associated with those sheets in NbS2as well.
In order to get information on the larger gap, it is nec-essary to perform a detailed analysis of the temperature dependence at higher temperature. The inset of fig.3 displays the temperature dependence of the-superfluid
Figure 2: Temperature dependence of the rescaled frequency shift δf /∆f0 ∝ ∆λab/λ0 in NbS2 at T<Tc/3 (red circles).
Results are fitted with the exponential low temperature ap-proximation (see text) to determine the smaller gap ∆. An excellent fit is obtained for ∆ ≈ 1.17 kBTc. Results can’t be
described by an exponential behaviour with the weak coupling BCS value ∆ = 1.76 kBTc. Inset: superconducting transition:
Tc=6.05 K is determined by the maximum of variation of the
density ˜ρab(T ) up to Tc deduced from Eq.(2) for
differ-ent R/λ0∆f0 values compared to Hf/Hf(0). Note that
if a small change in R/λ0∆f0 will modify strongly the
normalized superfluid density, the curvature of Hf(T) is
utterly independent of λ0. Hf(T) can hence be used to
determine R/λ0∆f0with good accuracy and, as shown, a
good agreement between Hfand the superfluid density is
obtained taking R/λ0∆f0= 0.02Hz−1. Clear deviations
from the BCS weak coupling theoretical curve (dashed line) is visible on the entire temperature range. In par-ticular, the BCS values exceed the experimental data at low temperature due to the small value of the gap.
In the multigap model, ˜ρ is phenomenologically as-sumed to be the sum of two independent superfluid den-sities
ρ = ω ˜ρ1+ (1 − ω) ˜ρ2 (4)
where ω is the weight of band 1 and ˜ρi are given by
˜ ρi(T ) = 1 − Z ∂f ∂E E pE2− ∆2 i(T ) (5) The best fit to the data using Eq.(4) and Eq.(5) (solid line in Fig.3) is obtained with ∆1= 1.05±0.05×kBTcand
∆2= 1.8 ± 0.1 × kBTc with ω ∼ 0.5. Those values are in
very good agreement with those deduced from tunneling spectroscopy measurements which revealed a distribution of gaps having two main values at 0.53 meV=6.15 K≈ 1 kBTcand 0.98 meV=10.8 K≈ 1.8 kBTc15. Moreover, the
Figure 3: Normalized superfluid density of NbS2
de-duced from Tunnel Diode Oscillator measurements (TDO) for Rλ0/∆f0=0.02Hz−
(closed squares), compared to Hf(T )/Hf(0)(open circles) both on sample C8. As shown,
the weak coupling BCS normalized superfluid density (dashed line) is not compatible with the data. A very similar tem-perature dependence was previously obtained in NbSe2 (solid
triangles) and both compounds could be well described by a two gap model (thick line, see text for details). Inset: influence of the R/λ0∆f0 parameter on the shape of the superfluid
den-sity, R/λ0∆f0 being equal to respectively 0.01, 0.02 and 0.03
Hz−1 for diamonds, squares and circles.
sample C8 can be well described taking ∆1∼ 1.05×kBTc,
∆2 ∼ 2.1 × kBTc and ω ∼ 0.616. Even if this two gap
model well reproduces the temperature dependence of ˜ρi
it is worth noting that this temperature dependence is also compatible with a single anisotropic in-plane super-conducting gap. The simplest model which respects the symmetry of the crystal has an in-plane 6-fold shape, ∆(φ) = ∆1+∆2−∆2 1(1 + cos(6φ)) where the extremum
of the superconducting gap define two characteristics en-ergy scales. With this model, we find ∆1∼ 0.9(1)× kBTc
and ∆2∼ 1.9(3) × kBTc.
IV. COMPARISON BETWEEN NBS2 AND
We have also reported in Fig.3 the temperature depen-dence of ˜ρab deduced from penetration depth
measure-ments in 2H-NbSe212. Since the critical temperatures
are slightly different in the two compounds, the data have been plotted as a function of T/Tcwith Tc= 6.05 K and
7.1 K for NbS2and NbSe2, respectively. In both case, the
presence of two characteristic gap values are necessary to fit the temperature dependence of the in-plane superfluid density. We hence show that in both compounds the ex-otic superconducting gap structure is related to the Nb tubular sheets and that, even if the charge density wave is
perturbing those sheets in NbSe2(but not in NbS2which
does not exhibit any CDW), this CDW does not affect the superconducting gap structure. Our results hence contradict the ARPES measurements on NbSe211which
suggested a strong correlation between the gap structure and the CDW formation. The presence of an identical exotic gap structure in two different compounds (even of the same family) is particularly rare which highlights the robustness of the underlying mechanism at its ori-gin. It’s worth noting that there exists a R/λ0∆f0value
(∼ 0.02Hz−1, see above) for which the temperature
de-pendence obtained on both compounds are very similar on the whole temperature range.
Note that this strong similitude in the gap structure is not in contradiction with the fact that the vortex cores have an isotropic shape in NbS215, and 6-fold shape in
NbSe232,33. Indeed, in this later case, the particular
shape could be due to an anisotropic Fermi velocity34
caused by the presence of the Charge Density Wave. Finally, It is interesting to note that even with sim-ilar superconducting gaps, it is possible to understand the large difference of the anisotropy of the upper crit-ical field in the two systems. In the case of NbSe2,
the anisotropy of the upper critical field can be under-stood by the anisotropy of the two set of Nb-bands. In-deed, the coherence length related to the pancake band is larger due to a large renormalised Fermi velocity and a small gap8. According to band structure calculations,
the anisotropy of the Fermi velocities (vab
F/vFc) of the two
tubular sheets are on the order of 2 (Band 1735) and 10
(Band 18) in NbSe2, none of which corresponding to the
experimental value of the anisotropy of the upper crit-ical field (∼ 3.2)23. However, µ
0Hc2kc(0) = Φ0/2πξab2 is
defined by the band having the smallest ξab value. All
bands have quite similar in plane Fermi velocities but if one assumes that ∆2 is associated with band 17 and ∆1
to band 18, on gets ξab,17 ∼ (∆1/∆2)ξab,18 ∼ ξab,18/1.7
c2 will be defined by band 17. Moreover, for
µ0Hc2kab(0) = Φ0/2πξabξc, and the very small value of
c-axis Fermi velocity of band 18, will imply that Hkab c2
will be defined by this latter band. One hence gets Hc2kab/H kc c2 = (v ab,17 F .v ab,17 F /v ab,18 F .v c,18 F ) × (∆1/∆2)2 ∼
10/(1.7)2 ∼ 3 in good agreement with the
experimen-tal value. Note that this situation strongly differs from the one observed in MgB2in which the anisotropy of Hc2
is defined only by the σ−band (for T << Tc). As NbSe2
and NbS2 have similar Hc2kab values, one can conclude
that band 18 is not affected by the chemical substitution and the increase of the Hc2 anisotropy to ∼ 8.1 in NbS2
is a hence due to an increase of vab,17
F but this change in
the Fermi velocity does not affect the superconducting gap structure.
The presence of two characteristics gap values appears to be a robust characteristic feature in 2H dichalco-genides, but its origin is still open to questions. With the present results, the influence of the CDW also has to be excluded, underlying the necessity to propose new 4
clues for the origin of the reduced superconducting gap observed in both compounds.
To conclude, the temperature dependence of the in-plane magnetic penetration depth of single crystals of 2H-NbS2 has been measured, and compared to previous
measurements on 2H-NbSe2. The temperature
depen-dence shows a similar curvature in both compounds evi-dencing a similar reduced superconducting gap structure in the sheets of the Fermi Surface where the e-ph
cou-pling constant are the largest. The CDW, present only in NbSe2, is not at the origin of the reduced
supercon-ducting gap. In the light of the discovery of a particular acoustic phonon mode observed in lead or Niobium36,
a more accurate knowledge of the phonon dispersion in NbS2 could shed insight into the origins of the reduced
superconducting gap in the dichalcogenides.
P.R. thanks R. and B. Thomas for helpful discussions. . TK is most obliged to V. Mosser of ITRON, Montrouge, and M.Konczykowski from the Laboratoire des Solides Ir-radiés, Palaiseau for the development of the Hall sensors used in this study
G. Seyfarth, J. P. Brison, and G. K. et al., Phys. Rev. Lett. 101, 046401 (2008).
E. Morosan, H. W. Zandbergen, and B. S. e. a. Dennis, Nature Physics 2, 544 (2006).
A.F. Kusmartseva, B. Sipos, H. Berger, L. Forro, E. Tutis, Phys. Rev. Lett. 103, 236401 (2009).
B. Sipos, A. Kusmartseva, and A. A. et al., Nature Mate-rials 7, 960 (2008).
K. E. Wagner, E. Morosan, Y. S. Hor, J. Tao, Y. Zhu, T. Sanders, T. M. McQueen, H. W. Zandbergen, A. J. Williams, D. V. West, et al., Phys. Rev. B 78, 104520 (2008).
P. Garoche, J. J. Veyssié, P. Manuel, and P. Molinié, Solid. State Comm. 19, 455 (1976).
H. F. Hess, R. B. Robinson, R. C. Dynes, J. M. Valles, and J. V. Waszczak, Phys. Rev. Lett. 62, 214 (1989).
R. Corcoran, P. Meeson, Y. Onuki, P. A. Probst, M. Springford, K. Takita, H. Harima, G. Y. Guo, and B. L. Gyorffy, J. Phys.: Condens. Matter 6, 4479 (1994).
D. Sanchez, A. Junod, J. Muller, H. Berger, and F. Lévy, Physica B 204, 167 (1995).
I. Guillamon, H. Suderow, F. Guinea, and S. Vieira, Phys. Rev. B 77, 134505 (2008).
T. Kiss, T. Yokoya, A. Chainani, S. Shin, T. Hanaguri, M. Nohara, and H. Takagi, Nat. Phys. 3, 720 (2007).
J. D. Fletcher, A. Carrington, P. Diener, P. Rodiere, J. P. Brison, R. Prozorov, T. Olheiser, and R. W. Giannetta, Phys. Rev. Lett. 98, 057003 (2007).
A. H. Castro Neto, Phys. Rev. Lett. 86, 4382 (2001).
S. V. Borisenko, A. A. Kordyuk, V. B. Zabolotnyy, D. S. Inosov, D. Evtushinsky, B. Büchner, A. N. Yaresko, A. Varykhalov, R. Follath, W. Eberhardt, et al., Phys. Rev. Lett. 102, 166402 (2009).
I. Guillamon, H. Suderow, S. Vieira, L. Cario, P. Diener, and P. Rodiere, Phys. Rev. Lett. 101, 166407 (2008).
J. Kacmarcik, Z. Pribulova, C. Marcenat, T. Klein, P. Rodiere, L. Cario, and P. Samuely, Phys. Rev. B 82, 014518 (2010).
R. Friend and A. D. Yoffe, Adv. Phys. 36, 1 (1987).
H. Suhl, B. T. Matthias, and L. R. Walker, Phys. Rev.
Lett. 3, 552 (1959).
H. Choi, D. Roundy, H. Sun, M. Cohen, L. Louie, and G. Steven, Nature 418, 758 (2002).
I. I. Mazin and V. P. Antropov, Physica C 385, 49 (2003).
T. Yokoya, T. Kiss, A. Chainani, and S. et al., Science 294, 2518 (2001).
E. Boaknin, M. A. Tanatar, J. Paglione, D. Hawthorn, F. Ronning, R. W. Hill, M. Sutherland, L. Taillefer, J. Sonier, S. M. Hayden, et al., Phys. Rev. Lett. 90, 117003 (2003).
M. D. Johannes, I. I. Mazin, and C. A. Howells, Phys. Rev. B 73, 205102 (2006).
K. Onabe, M. Naito, and S. Tanaka, J. Phys. Soc. Jpn. 45, 50 (1978).
W. Fisher and M. Sienko, Inorg. Chem. 19, 39 (1980).
C. Van Degrift, Rev. Sci. Instrum. 46, 599 (1975).
P. Diener, P. Rodiere, T. Klein, C. Marcenat, J. Kacmar-cik, Z. Pribulova, D. J. Jang, H. S. Lee, H. G. Lee, and S. I. Lee, Phys. Rev. B 79, 220508 (2009).
R. Prozorov, R. W. Giannetta, A. Carrington, P. Fournier, R. L. Greene, P. Guptasarma, D. G. Hinks, and A. R. Banks, Appl. Phys. Lett. 77, 4202 (2000).
R. Prozorov, R. W. Giannetta, A. Carrington, F.M. Araujo-Moreira Phys. Rev. B 62, 115 (2000).
T. Klein, D. Braithwaite, A. Demuer, Phys. Rev. B 82, 184506 (2010).
B. Chandrasekhar and D. Einzel, Ann. Phys. 505, 535 (1993).
H. F. Hess, R. B. Robinson, and J. V. Waszczak, Phys. Rev. Lett. 64, 2711 (1990).
I. Guillamon, H. Suderow, S. Vieira, and P. Rodiere, Phys-ica C 468, 537 (2008).
F. Gygi and M. Schluter, Phys. Rev. Lett. 65, 1820 (1990).
the two set of Nb-bands called by Corcoran et al. 17 and 18, correspond respectively to 2 and 3 in Johannes and Mazin
P. Aynajian, T. Keller, L. Boeri, S. M. Shapiro, K. Habicht, and B. Keimer, Science 319, 1509 (2008).